Cite as: APL Mater. 8, 061102 (2020); https://doi.org/10.1063/5.0010233
Submitted: 09 April 2020 . Accepted: 14 May 2020 . Published Online: 02 June 2020
Vibrational properties of LaNiO
in the ultrathin regime
Cite as: APL Mater. 8, 061102 (2020);doi: 10.1063/5.0010233
Submitted: 9 April 2020 • Accepted: 14 May 2020 • Published Online: 2 June 2020
Alexander Schober,1,2 Jennifer Fowlie,3 Mael Guennou,1,2 Mads C. Weber,4 Hongjian Zhao,1,5 Jorge Íñiguez,1,2 Marta Gibert,6 Jean-Marc Triscone,3 and Jens Kreisel1,2
1Materials Research and Technology Department, Luxembourg Institute of Science and Technology, 41 rue du Brill, L-4422 Belvaux, Luxembourg
2Department of Physics and Materials Science, University of Luxembourg, 41 rue du Brill, L-4422 Belvaux, Luxembourg 3DQMP – University of Geneva, École de Physique, 24, Quai Ernest-Ansermet, CH-1211 Geneva, Switzerland
4Department of Materials, ETH Zurich, Vladimir-Prelog-Weg 4, 8093 Zurich, Switzerland
5Physics Department and Institute for Nanoscience and Engineering University of Arkansas, Fayetteville, Arkansas 72701, USA 6Physik-Institut, University of Zurich, Winterthurerstrasse 190, 8057 Zurich, Switzerland
Collective rotations and tilts of oxygen polyhedra play a crucial role in the physical properties of complex oxides such as magnetism and con-ductivity. Such rotations can be tuned by preparing thin films in which dimensionality, strain, and interface effects come into play. However, little is known of the tilt and rotational distortions in films a few unit cells thick including the question of if coherent tilt patterns survive at all in this ultrathin limit. Here, a series of films of perovskite LaNiO3is studied and it is shown that the phonon mode related to oxygen
octahedral tilts can be followed by Raman spectroscopy down to a film thickness of three pseudocubic perovskite unit cells (∼1.2 nm). To push the limits of resolution to the ultrathin regime, a statistical analysis method is introduced to separate the Raman signals of the film and substrate. Most interestingly, these analyses reveal a pronounced hardening of the tilt vibrational mode in the thinnest films. A comparison between the experimental results, first principles simulations of the atomic structure, and the standing wave model, which accounts for size effects on the phononic properties, reveals that in the ultrathin regime, the Raman spectra are a hybrid entity of both the bulk and surface phononic behavior. These results showcase Raman spectroscopy as a powerful tool to probe the behavior of perovskite films down to the ultrathin limit.
© 2020 Author(s). All article content, except where otherwise noted, is licensed under a Creative Commons Attribution (CC BY) license (http://creativecommons.org/licenses/by/4.0/).https://doi.org/10.1063/5.0010233., s
Physical properties of complex oxides are remarkably sen-sitive to minute details of their crystal structure.1,2 In particu-lar, rotations or tilts of the oxygen polyhedra govern the orbital overlap between cations and oxygen-anions and can determine magnetism, electronic conductivity, metal–insulator transitions, or ferroelectricity, as a few examples.3,4In rare-earth nickelates, struc-tural tuning by heterostructuring has been shown to cause remark-able shifts in transition temperatures through the modulation of the orbital overlaps.5,6 While biaxial strain tends to extend over
tens of nanometers, octahedral tilts in perovskite oxide heterostruc-tures can vary over single unit cell layers.7–13 At an interface, par-ticularly, strong variations can occur, opening up the possibility to design functional heterostructures. For instance, it was previously demonstrated that LaNiO3 films on the (001)pc-oriented LaAlO3
thickness-dependent, detailed modeling of x-ray diffraction signals has shown that the film-averaged octahedral tilts and rotations of LaNiO3on LaAlO3are robust and remain unchanged in magnitude
down to 5 pc u.c.17
A further experimental technique that has been successfully applied to investigate the structure of thin films and heterostructures is Raman spectroscopy.18–21Raman spectroscopy has major advan-tages over the techniques mentioned already: It is non-destructive and does not require large facilities. Furthermore, Raman spec-troscopy allows the structural order to be traced via the so-called soft mode.22This soft-mode spectroscopy approach was previously employed in, for instance, bulk LaAlO323–25and SrTiO326to follow
tilt distortions. In contrast to polar soft modes correlated with fer-roelectricity,20 there is, to the best of the authors’ knowledge, no experimental data on how soft tilt modes behave for ultrathin films. The aim of this work is an in-depth understanding of tilt distor-tions in the ultrathin limit and how the corresponding Raman spec-trum relates to these structural details, as the thickness is decreased from a usually well-known bulk spectrum to a two-dimensional system.
Here, LaNiO3films of different thicknesses on the LaAlO3
sub-strate in (001)pcpseudocubic orientation [Fig. 1(a)] are investigated
by Raman spectroscopy. Both the bulk LaNiO3 and the LaAlO3
substrate are ABO3perovskites with the same rhombohedral space
group,R3c, and tilt system, written as a−a−a−in Glazer notation.
Both compounds have antiphase octahedral tilts of equal magnitude (5.6○in LaAlO
3and 5.2○in LaNiO327,28) about the three
pseudocu-bic directions that can be compounded into one antiphase rotation magnitude around the pcvector.29Figure 1(b)displays the thick
film Raman spectrum for LaNiO3and the bulk Raman spectrum for
the substrate LaAlO3. In LaNiO3, the octahedral rotation distortion,
the order parameter of the system, is related to the only fully sym-metricA1gphonon mode19,30–32sketched inFig. 1(c). TheA1gmode
is, therefore, described as a “soft mode.” The softening of this mode with increasing temperature was evidenced in Ref.31, in relation to a transition to the cubic phase that is not observed in practice but would occur at about 1780 K.
OF ULTRATHIN FILMS
A major challenge for Raman spectroscopy on very thin films is the predominant signal of the substrate. Here, this issue is overcome by employing a specific strategy, combining confocal micro-Raman spectroscopy and principal component analysis (PCA) to extract the weak phonon signal from the films by demixing the depth-resolved spectra. The basic setup is schematized inFig. 2(a). The signal of the film and the signal of the substrate have different depth dependen-cies. The film signal is the strongest for a laser focus in the vicinity of the surface, whereas the substrate signal remains strong for a laser focus deep into the sample, as sketched on the right ofFig. 2(a). These distinct evolutions with the laser focus allow the separation of film and substrate signals by multivariate analysis methods.33Here, principal component analysis (PCA) was used to treat the data. This analysis generates three important parameters—(a) The principal components: A set of individual spectra that describe the features of the measured stack of data. (b) The eigenvalues of the principal com-ponents: The larger the value, the more important the corresponding component for the dataset. (c) The score of the components: The score shows an evolution of the weight of a principal component throughout the dataset. The image inFig. 2(b)shows an applica-tion of the method for a 7 pc u.c. (2.7 nm) LaNiO3sample, where
the laser focal pointz is varied within ±10 μm of the sample sur-face in 0.2 μm steps. The eigenvalues obtained from the PCA are shown inFig. 2(c). As can be seen, only the first two components have a significant weight and are relevant for the analysis (indicated by the blue and red squares). All other components have a very small variance and can be treated as negligible. The scores of these two components are shown inFig. 2(d)and have a distinct behav-ior as a function ofz, being step-like and peak-shaped, respectively. The corresponding components are displayed inFig. 2(e)and com-pared with the raw spectrum. As anticipated, the first component can be associated with the substrate spectrum and shows the peaks known from LaAlO3[seeFig. 1(b)], while the second component
is associated with the film spectrum, where the characteristic peaks are clearly distinguished. Especially remarkable is the demixing of
FIG. 1. (a) Sketch of the LaNiO3
lay-ers on -oriented LaAlO3 with the
pseudocubic unit cell (pc u.c.) indicated. (b) Raman spectra of a thick polycrys-talline LaNiO3 film and a LaAlO3
sub-strate. (c) Atomic displacement patterns of the LaNiO3 Raman modes shown
in (b), where the single A1g soft mode
FIG. 2. (a) Simplified sketch of the experimental conditions and the probed volume during the micro-Raman experiment alongside the expected depth dependence of the
film and substrate components (not to scale). (b) Full depth measurement dataset for 7 pc u.c. of LaNiO3on LaAlO3. (c) Singular value decomposition of the data shown
in (b), indicating two major components indicated by the blue and red squares. (d) Principal component analysis (PCA) scores obtained on the same data for the first two components. (e) Final PCA components obtained from the depth-dependent dataset shown in (b) with the raw Raman spectrum recorded at the depth of highest film intensity (black).
the substrate and film peaks at 210–230 cm−1. As can be seen, this method allows the separation of the film and substrate spectra and extraction of detailed film information undisturbed by the substrate signal.
Earlier studies using depth-dependent confocal Raman spec-troscopy on oxide thin films rely on the subtraction of the substrate signal.21,34Such a subtraction is based on the assumption that the spectral signature of the substrate is uniform. However, substrate responses are often modified at interfaces and between domains. Thus, a subtraction risks the introduction of artifacts. The statisti-cal treatment of the present work compensates for varying substrate responses and allows for a clean separation of the substrate and film signal.
As displayed inFig. 2, two Raman modes of the LaNiO3films
are accessible in this frequency range: theA1g mode and oneEg
mode, corresponding to tilts and bending of the BO6 octahedra
[Fig. 1(c)]. The soft mode of interest is the only fully symmetric mode withA1g symmetry. The mode notations relate here to the
bulk rhombohedral symmetry, even though it is known that epitaxial strain stabilizes a monoclinic structureC2/c (a−a−c−), as revealed by
density functional theory (DFT) and Raman spectroscopy on films down to 14 nm.19The symmetry lowering leads to the splitting of EgRaman peaks as well as the emergence of new peaks, but for
sim-plicity, the labeling with respect to the bulk will be retained in this discussion.
THICKNESS DEPENDENCE OF THE RAMAN MODES We now apply the same measurement and analysis method to the full series of nine LaNiO3films with thicknesses ranging from
3 pc u.c. to 15 pc u.c., as verified by x-ray diffraction and scan-ning transmission electron microscopy. Three representative spectra for 11 pc u.c., 7 pc u.c., and 3 pc u.c. are showcased inFig. 3(a). Three fits associated with the film component of the data shown in
FIG. 3. (a) Raw Raman spectra of LaNiO3on LaAlO3for 3 pc u.c., 7 pc u.c., and 11 pc u.c. The spectra were chosen from the depth where the film signal is maximal. (b)
Film components extracted from the PCA with the A1gand Egpeaks sketched in red and blue, respectively. The additional peaks resulting from the symmetery-lowering are sketched as dashed lines. (c) Position and half width at half maximum (HWHM) of the LaNiO3Egand A1gmodes resulting from the fits for the entire series of samples. Solid
lines show an exponential decay fit to the data.
shoulders, shown as dotted lines inFig. 3(b), will not be discussed further.
Figure 3(c) shows the resulting peak positions as well as the half width at half maximum (HWHM) for the A1g mode (top)
and Eg mode (bottom) described above for the entire series of
LaNiO3films with varying thickness. Both modes show a
qualita-tively similar behavior with two different regimes. For films thicker than 15 u.c., both the positions and widths are constant and coin-cide with the values reported in previous studies.19 As thickness decreases, the mode frequency and width enter a second regime and both exhibit a pronounced increase.Figure 3(c)shows a fit of this behavior with an exponential evolution. The critical thicknesses are 8–10 u.c. (3–4 nm), and notably, the mode frequency increases for lower thicknesses, i.e., moves away from the corresponding soft mode of LaAlO3, which is at lower frequency, as shown in
Fig. 1(b), in accordance with reports on theEgmode by Hepting and
ESTIMATE OF THE RAMAN FREQUENCIES BY FIRST-PRINCIPLES
In order to provide a more thorough understanding of the Raman signature and its relation with the structure of the film, a theoretical model was constructed. Within this model, an esti-mate of the soft-mode frequency can be obtained directly by start-ing from the relaxed film structures reported previously.11 These structures were obtained by running first-principles simulations in which finite LaNiO3films of different thicknesses and the LaAlO3
substrate were treated explicitly. Then, the equilibrium solutions are distorted by moving the oxygen atoms within the LaNiO3film
so as to mimic antiphase rotations of the O6octahedra about the
pcaxis. From this, the harmonic energy variation is computed.
The energy curvature κsoftis thus obtained, and the mode frequency
can be approximated as ωsoft =
κsoft/mO, wheremOis the mass
of the oxygen ion. It is assumed that the eigenvector of the soft tilting mode of thea−a−c−-type monoclinic films can be
approxi-mated by the well-known symmetry-determinedA1g eigenmode of
the bulk crystal.
The results of the first-principles approach are shown in
Fig. 4(a). Compared to the Raman spectra, here, a similar soft mode hardening on the order of 20 cm−1is observed. The critical thickness where the mode hardening sets in is slightly reduced in the theory compared to the experiment (5 u.c. compared to 10 u.c.). These first principles calculations based on the microscopic structure, there-fore, provide a reasonable description of the mode hardening in ultrathin films.
STANDING WAVE APPROXIMATION
FIG. 4. (a) Comparison of the experimental value for the A1gsoft mode frequency
(red circles), together with the same parameter derived from direct first principles calculation (blue diamonds) and the standing wave approach (green squares). The dashed lines are guides for the eye. (b) Phonon dispersion of bulk LaNiO3along
the  direction in the wavelength range of interest.
non-polar. As a result, the electrostatic boundary conditions and the dielectric properties of the media are not relevant here. Following the ideas developed in Ref.36, we assume that non-polar modes will behave like transverse optical modes propagating perpendicular to the films, that is, without any polar component along the direc-tion of the wavevector. The frequency of the phonon in the film is then approximated as the frequency calculated in the bulk on this phonon branch at a wavevector π/d, where d is the number of pseu-docubic unit cells in the film. With changing film thickness, the wavevector and the frequency change according to the dispersion relation.40The boundary conditions for the approximation are rep-resented by a wave amplitude vanishing at the interfaces. In other words, the phonon cannot propagate across the interface due to a large mismatch between the phonon frequencies of the two media.41 In practice, the phonon dispersion for bulk LaNiO3, shown in
Fig. 4(b), was calculated from first principles and the soft branch fol-lowed across the Brillouin zone. Given the complexity of the phonon dispersion relation, care was taken to follow the correct phonon branch originating from theA1g tilt mode by checking the branch
symmetry and the phonon eigenvector. As a result of the posi-tive slope of the phonon branch, the soft mode frequency in the films increases as the size effect becomes more significant toward the ultrathin regime, reproducing the trend from experiment. As compared to the mode hardening seen in the Raman spectra, both the critical thickness for the hardening and the overall increase in frequency are greater. Part of this discrepancy may be due to the interface between the LaNiO3 film and the LaAlO3 substrate
not establishing a sharp boundary condition—as both materials are similar in crystal structure, structural instabilities, and phonon spectrum—and, thus, reducing the effective size effect in practice. DISCUSSION
These Raman spectroscopy investigations into the ultrathin regime of LaNiO3on the LaAlO3substrate have brought to light a
number of intriguing behaviors. Importantly, owing to the advanced
technical and analytical approaches employed here, both the soft phonon mode associated with the tilts and the octahedral bending mode remained measurable by Raman spectroscopy down to 3 pc u.c. (1.2 nm)—a thickness around which the distorted unit cell itself is almost undefined. Both theA1g and theEg modes show a very
similar hardening beginning below 10 pc u.c.
This picture differs from a number of conventional interpre-tations of Raman spectra of thin films. In particular, the possibility that the shifts of Raman modes are due to a relaxation of epitaxial strain was put forward in a previous study on theEgbending mode
of LaNiO3films34 but can be ruled out here as all the films
stud-ied were epitaxially strained to the substrate. Moreover, as the global LaNiO3octahedral rotations and tilts were found, by x-ray
diffrac-tion, not to vary with thickness down to 5 pc u.c.,17it appears that, in contrast with bulk systems, theA1gmode frequency no longer scales
linearly with the tilt angle. However, the bulk linear scaling follows a slope on the order of 20–30 cm−1/○in the similarly structured
chro-mates and ferrites.42,43This suggests that the tilt could increase by as little as one degree toward the ultrathin limit, which would be within the experimental error of the x-ray diffraction signal fitting reported previously.
On the other hand, it is remarkable that the two observed modes—both bending and tilting—of LaNiO3exhibit very similar
hardenings, with the same critical thickness, and shifts of nearly equal amplitudes. The standing wave approach employed here par-tially explains this behavior as both modes have an increase in fre-quency when moving away from the zone center. Therefore, the observation that both our Raman modes undergo a similar harden-ing is likely to be material-dependent. Recent reports on ultrathin BaTiO3 films40 show a contrasting behavior for different modes.
This underlines that the vibrational frequencies in the ultrathin limit indeed depend on the mode details and dispersion. The frequency increase in LaNiO3that is predicted by the standing wave approach
is, however, greater in magnitude than that observed in practice, but as discussed, this could stem from vibrational continuity into the substrate.
A comparison with the first-principles results shows that a purely microscopic simulation of the soft mode frequency can go a reasonable way to reproducing the same hardening behavior. As found previously by first-principles calculations and corroborated by experiment,11the LaNiO3surface tends to dominate the
over-all properties toward the ultrathin limit. Ultimately, for the thinnest films, the energy variation—and, therefore, the Raman frequency— is determined by a region of the film that is relatively stiff against the NiO6tilting mode. The complete thickness-dependence is not
fully described in this picture, however, with the onset of the mode hardening taking place at 10 pc u.c. in the experiment.
The experimental mode hardening follows a trend that is part way between that predicted by the direct first-principles estimate and that predicted by the standing wave approximation. This leads toward the natural conclusion that, in this ultrathin regime, the thin film cannot be considered as simply a slice of the bulk crystal but rather as a hybrid entity. Therefore, discussion of both the phononic behavior of a crystalline solid and the vibrational properties of a surface is required.
in more complex systems—in terms of symmetry and number of modes—than LaNiO3 on the LaAlO3substrate. Interestingly, the
change in metallicity due to the altered film thicknesses11does not impact the quality of the PCA. This further underlines the universal-ity of our approach. Modes corresponding to the oxygen octahedral tilting and bending could still be identified in films as thin as 3 pseu-docubic unit cells or 1.2 nm—a testament both to the power of the analysis technique and to the high quality of the thin films. Both of these modes are found to harden significantly toward the atomic limit. The onset of the hardening cannot be fully accounted for by microscopic considerations alone. Incorporating a standing wave approach, commonly employed in the study of surface vibrations, sheds light on the possibility of an unexpected phononic behavior in this pseudo-2D regime that should be general to ultrathin films as a whole.
The samples were grown by radio frequency off-axis magnetron sputtering at a temperature of 510○C and a pressure of 0.18 mTorr
(Ar:O27:2 mix). The series ranges from 3 to 15 unit cells. The films
were characterized by x-ray diffraction, atomic force microscopy, and scanning transmission electron microscopy and were found to be coherently strained, with an atomically flat surface and high crystalline quality.11
The experiments were performed, at room temperature, with a Renishaw inVia micro-Raman spectrometer. The excitation wave-length was 633 nm, with laser power lower than 1 mW. The exciting light is focused via a ×100 microscope objective with numerical aper-ture 0.9, resulting in nominal spot size and depths of the field of 0.86 μm and 1.38 μm, respectively. The scattered light was analyzed with a holographic grating with 2400 g/mm and collected on a CCD detector. All data treatments (principal component analysis and fit-ting with standard Lorentzian line shapes) were performed with a python-based software developed in house.
Ab initio calculation details
We used density functional theory (DFT) as within the local density approximation (LDA), as implemented in the Vienna ab initio simulation package (VASP).44,45 We treated the ionic cores within the so-called projector-augmented wave (PAW) approach,46 solving explicitly for the following electrons: La 5p, 5d, and 6s; Ni 3p, 3d, and 4s; Al 3s and 3p; and O 2s and 2p. The 3d electrons of Ni were treated at the bare LDA level, which has been shown to be the most realistic way to treat metallic LaNiO3.47Details about
the structures combining the LaNiO3 film and LaAlO3 substrate
are described in some detail in Ref.11. For our phonon calcula-tions for bulk LaNiO3, we used the usual 10-atom primitive cell
of this compound. Electronic wave functions were represented in a plane-wave basis truncated at 400 eV and 500 eV, respectively, for our LaNiO3/LaAlO3(001) and bulk LaNiO3simulations. Reciprocal
space integrals were computed using a 5 × 5 × 1k-point mesh in
points was used to treat bulk LaNiO3in its 10-atom primitive cell.
We used phonopy48for the calculation of phonon bands, using a 2 × 2 × 2 multiple of the 10-atom primitive cell (and, correspondingly, a 4 × 4 × 4k-point grid).
J.F. fabricated and characterized the samples. A.S. performed the Raman experiments and developed the tools for their analysis with input from M. Guennou. M.C.W. initiated the use of a multi-variate analysis method to study ultrathin films. H.Z. and J.I. per-formed and analyzed the DFT calculations. J.-M.T. and J.K. directed the research. All authors contributed to the analysis of the results and the preparation of this manuscript.
A.S., M. Guennou, H.Z., J.I., and J.K. acknowledge sup-port from the Luxembourg National Research Fund under Project No. CO-FERMAT FNR/P12/4853155/Kreisel and the AFR, Grant No. 7749159. M.C.W. acknowledges support from SNSF (Grant No. 200021_178825). M. Gibert acknowledges financial support through the SNSF, Grant No. PP00P2_170564. This work was supported by the Swiss National Science Foundation through Division II. The research leading to these results has received funding from the Euro-pean Research Council under the EuroEuro-pean Union’s Seventh Frame-work Program (No. FP7/2007-2013)/ERC Grant Agreement No. 319286 (Q-MAC). M. Guennou also gratefully acknowledges dis-cussion and input from W. Widdra (MPI of Microstructure Physics, Halle, Germany).
The data that support the findings of this study are available from the corresponding author upon reasonable request.
R. H. Mitchell,Perovskites: Modern and Ancient (Almaz Press, Ontario, Canada, 2002).
2J. B. Goodenough, “Electronic and ionic transport properties and other physical
aspects of perovskites,”Rep. Prog. Phys.67, 1915 (2004).
J. M. Rondinelli, S. J. May, and J. W. Freeland, “Control of octahedral connec-tivity in perovskite oxide heterostructures: An emerging route to multifunctional materials discovery,”MRS Bull.37, 261–270 (2012).
J. Nordlander, M. Campanini, M. D. Rossell, R. Erni, Q. N. Meier, A. Cano, N. A. Spaldin, M. Fiebig, and M. Trassin, “The ultrathin limit of improper ferroelectricity,”Nat. Commun.10, 5591 (2019).
S. Catalano, M. Gibert, J. Fowlie, J. Íñiguez, J.-M. Triscone, and J. Kreisel, “Rare-earth nickelates RNiO3: Thin films and heterostructures,”Rep. Prog. Phys.81,
S. Middey, J. Chakhalian, P. Mahadevan, J. W. Freeland, A. J. Millis, and D. D. Sarma, “Physics of ultrathin films and heterostructures of rare-earth nickelates,”
Annu. Rev. Mater. Res.46, 305–334 (2016).
W. Lu, W. Song, P. Yang, J. Ding, G. M. Chow, and J. Chen, “Strain engineering of octahedral rotations and physical properties of SrRuO3films,”Sci. Rep.5, 10245
Z. Liao, M. Huijben, Z. Zhong, N. Gauquelin, S. Macke, R. J. Green, S. Van Aert, J. Verbeeck, G. Van Tendeloo, K. Held, G. A. Sawatzky, G. Koster, and G. Rijnders, “Controlled lateral anisotropy in correlated manganite heterostruc-tures by interface-engineered oxygen octahedral coupling,”Nat. Mater.15, 425 (2016).
D. Kan, R. Aso, R. Sato, M. Haruta, H. Kurata, and Y. Shimakawa, “Tun-ing magnetic anisotropy by interfacially engineer“Tun-ing the oxygen coordination environment in a transition metal oxide,”Nat. Mater.15, 432 (2016).
11J. Fowlie, M. Gibert, G. Tieri, A. Gloter, J. Íñiguez, A. Filippetti, S. Catalano,
S. Gariglio, A. Schober, M. Guennou, J. Kreisel, O. Stéphan, and J.-M. Triscone, “Conductivity and local structure of LaNiO3thin films,”Adv. Mater.29, 1605197
A. Y. Borisevich, H. J. Chang, M. Huijben, M. P. Oxley, S. Okamoto, M. K. Niranjan, J. D. Burton, E. Y. Tsymbal, Y. H. Chu, P. Yu, R. Ramesh, S. V. Kalinin, and S. J. Pennycook, “Suppression of octahedral tilts and associated changes in electronic properties at epitaxial oxide heterostructure interfaces,”Phys. Rev. Lett.
105, 087204 (2010).
A. Vailionis, H. Boschker, Z. Liao, J. R. A. Smit, G. Rijnders, M. Huijben, and G. Koster, “Symmetry and lattice mismatch induced strain accommodation near and away from correlated perovskite interfaces,”Appl. Phys. Lett.105, 131906 (2014).
R. Scherwitzl, S. Gariglio, M. Gabay, P. Zubko, M. Gibert, and J.-M. Triscone, “Metal-insulator transition in ultrathin LaNiO3 films,” Phys. Rev. Lett.106,
J. Son, P. Moetakef, J. M. LeBeau, D. Ouellette, L. Balents, S. J. Allen, and S. Stemmer, “Low-dimensional Mott material: Transport in ultrathin epitaxial LaNiO3films,”Appl. Phys. Lett.96, 062114 (2010).
D. P. Kumah, A. S. Disa, J. H. Ngai, H. Chen, A. Malashevich, J. W. Reiner, S. Ismail-Beigi, F. J. Walker, and C. H. Ahn, “Tuning the structure of nickelates to achieve two-dimensional electron conduction,”Adv. Mater.26, 1935–1940 (2014).
J. Fowlie, C. Lichtensteiger, M. Gibert, H. Meley, P. Willmott, and J.-M. Triscone, “Thickness-dependent perovskite octahedral distortions at heterointer-faces,”Nano Lett.19, 4188–4194 (2019).
J. Kreisel, M. C. Weber, N. Dix, F. Sánchez, P. A. Thomas, and J. Fontcuberta, “Probing individual layers in functional oxide multilayers by wavelength-dependent Raman scattering,”Adv. Funct. Mater. 22, 5044–5049 (2012).
19M. C. Weber, M. Guennou, N. Dix, D. Pesquera, F. Sánchez, G. Herranz,
J. Fontcuberta, L. López-Conesa, S. Estradé, F. Peiró, J. Íñiguez, and J. Kreisel, “Multiple strain-induced phase transitions in LaNiO3thin films,”Phys. Rev. B94,
20D. A. Tenne, A. Bruchhausen, N. D. Lanzillotti-Kimura, A. Fainstein, R. S.
Kati-yar, A. Cantarero, A. Soukiassian, V. Vaithyanathan, J. H. Haeni, W. Tian, D. G. Schlom, K. J. Choi, D. M. Kim, C. B. Eom, H. P. Sun, X. Q. Pan, Y. L. Li, L. Q. Chen, Q. X. Jia, S. M. Nakhmanson, K. M. Rabe, and X. X. Xi, “Probing nanoscale ferroelectricity by ultraviolet Raman spectroscopy,”Science313, 1614 (2006).
21M. Hepting, M. Minola, G. Cristiani, G. Logvenov, E. Schierle, M. Wu,
M. Bluschke, E. Weschke, H.-U. Habermeier, E. Benckiser, M. Le Tacon, and B. Keimer, “Tunable charge and spin order in PrNiO3thin films and superlattices,” Phys. Rev. Lett.113, 227206 (2014).
J. F. Scott, “Soft-mode spectroscopy: Experimental studies of structural phase transitions,”Rev. Mod. Phys.46, 83 (1974).
J. F. Scott, “Raman study of trigonal-cubic phase transitions in rare-earth aluminates,”Phys. Rev.183, 823 (1969).
24S. A. Hayward, F. D. Morrison, S. A. T. Redfern, E. K. H. Salje, J. F. Scott, K. S.
Knight, S. Tarantino, A. M. Glazer, V. Shuvaeva, P. Daniel, M. Zhang, and M. A. Carpenter, “Transformation processes in LaAlO3: Neutron diffraction, dielectric,
thermal, optical, and Raman studies,”Phys. Rev. B72, 054110 (2005).
P. Bouvier and J. Kreisel, “Pressure-induced phase transition in LaAlO3,” J. Phys.: Condens. Matter14, 3981 (2002).
26P. A. Fleury, J. F. Scott, and J. M. Worlock, “Soft phonon modes and the 110 K
phase transition in SrTiO3,”Phys. Rev. Lett.21, 16–19 (1968). 27
K. A. Müller, W. Berlinger, and F. Waldner, “Characteristic structural phase transition in perovskite-type compounds,”Phys. Rev. Lett.21, 814 (1968).
28J. L. García-Muñoz, J. Rodríguez-Carvajal, P. Lacorre, and J. B. Torrance,
“Neutron-diffraction study of RNiO3(R = La, Pr, Nd, Sm): Electronically induced
structural changes across the metal-insulator transition,”Phys. Rev. B46, 4414 (1992).
A. M. Glazer, “Simple ways of determining perovskite structures,”Acta Crystal-logr., Sect. A31, 756 (1975).
30M. V. Abrashev, A. P. Litvinchuk, M. N. Iliev, R. L. Meng, V. N. Popov, V. G.
Ivanov, R. A. Chakalov, and C. Thomsen, “Comparative study of optical phonons in the rhombohedrally distorted perovskites LaAlO3and LaMnO3,”Phys. Rev. B
59, 4146–4153 (1999).
N. Chaban, M. Weber, S. Pignard, and J. Kreisel, “Phonon Raman scattering of perovskite LaNiO3thin films,”Appl. Phys. Lett.97, 031915 (2010).
32G. Gou, I. Grinberg, A. M. Rappe, and J. M. Rondinelli, “Lattice normal modes
and electronic properties of the correlated metal LaNiO3,”Phys. Rev. B84, 144101
33J. Kunc, Y. Hu, J. Palmer, C. Berger, and W. A. de Heer, “A method to extract
pure Raman spectrum of epitaxial graphene on SiC,”Appl. Phys. Lett.103, 201911 (2013).
34M. Hepting, D. Kukuruznyak, E. Benckiser, M. Le Tacon, and B. Keimer,
“Raman light scattering on ultra-thin films of LaNiO3under compressive strain,” Physica B460, 196–198 (2015).
35G. Benedek and J. P. Toennies, “Helium atom scattering spectroscopy of surface
phonons: Genesis and achievements,”Surf. Sci.299-300, 587–611 (1994).
P. Senet, P. Lambin, and A. A. Lucas, “Standing-wave optical phonons confined in ultrathin overlayers of ionic materials,”Phys. Rev. Lett.74, 570–573 (1995).
37L. Savio, E. Celasco, L. Vattuone, M. Rocca, and P. Senet, “MgO/Ag(100):
Con-fined vibrational modes in the limit of ultrathin films,”Phys. Rev. B67, 075420 (2003).
38V. Goian, F. O. Schumann, and W. Widdra, “Growth and lattice
dynam-ics of ultrathin BaO films on Pt(001),”J. Phys.: Condens. Matter30, 095001 (2018).
39L. Vattuone, L. Savio, and M. Rocca, “Phonons in thin oxide films,” inOxide
Materials at the Two-Dimensional Limit (Springer, 2016), pp. 169–199.
J. Premper, F. O. Schumann, A. Dhaka, S. Polzin, K. L. Kostov, V. Goian, D. Sander, and W. Widdra, “Surface stress and lattice dynamics in oxide ultrathin films,”Phys. Status Solidi B(published online 2020).
B. K. Ridley,Electrons and Phonons in Semiconductor Multilayers (Cambridge University Press, 2009).
42M. C. Weber, J. Kreisel, P. A. Thomas, M. Newton, K. Sardar, and R. I. Walton,
“Phonon Raman scattering of RCrO3perovskites (R = Y, La, Pr, Sm, Gd, Dy, Ho,
Yb, Lu),”Phys. Rev. B85, 054303 (2012).
43M. C. Weber, M. Guennou, H.-J. Zhao, J. Iniguez, R. Vilarinho, A. Almeida, J. A.
Moreira, and J. Kreisel, “Raman spectroscopy of rare-earth orthoferrites RFeO3(R
= La, Sm, Eu, Gd, Tb, Dy),”Phys. Rev. B94, 214103 (2016).
44G. Kresse and J. Furthmüller, “Efficient iterative schemes forab initio
total-energy calculations using a plane-wave basis set,”Phys. Rev. B54, 11169–11186 (1996).
45G. Kresse and D. Joubert, “From ultrasoft pseudopotentials to the projector
augmented-wave method,”Phys. Rev. B59, 1758–1775 (1999).
P. E. Blöchl, “Projector augmented-wave method,”Phys. Rev. B50, 17953– 17979 (1994).
47M. Gibert, P. Zubko, R. Scherwitzl, J. Íñiguez, and J.-M. Triscone, “Exchange
bias in LaNiO3–LaMnO3superlattices,”Nat. Mater.11, 195–198 (2012). 48